LMucko/crystallography-open-database huggingface dataset:
Halite-sylvite thermoelasticity Sample: r53261, T = 475 C, P = 12.1 kbar, cell volume = 234.59 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003152
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r53261, T = 475 C, P = 12.1 kbar, cell volume = 234.59 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.1674
_cell_length_b                   6.1674
_cell_length_c                   6.1674
_cell_volume                     234.588
_cell_formula_units_Z            4
_database_code_amcsd             0003241
_diffrn_ambient_pressure         1.21e+06
_diffrn_ambient_temperature      748.15
_exptl_crystal_density_diffrn    2.020
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003152
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: als7k80, T = 500 C, P = 0.0 kbar, cell volume = 251.33 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003153
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als7k80, T = 500 C, P = 0.0 kbar, cell volume = 251.33 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.3108
_cell_length_b                   6.3108
_cell_length_c                   6.3108
_cell_volume                     251.335
_cell_formula_units_Z            4
_database_code_amcsd             0003242
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    1.885
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003153
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: r55617, T = 500 C, P = 7.0 kbar, cell volume = 241.37 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003154
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r55617, T = 500 C, P = 7.0 kbar, cell volume = 241.37 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.2263
_cell_length_b                   6.2263
_cell_length_c                   6.2263
_cell_volume                     241.374
_cell_formula_units_Z            4
_database_code_amcsd             0003243
_diffrn_ambient_pressure         7e+05
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    1.963
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003154
Halite-sylvite thermoelasticity Sample: r55577, T = 500 C, P = 9.6 kbar, cell volume = 236.99 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003155
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r55577, T = 500 C, P = 9.6 kbar, cell volume = 236.99 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.1884
_cell_length_b                   6.1884
_cell_length_c                   6.1884
_cell_volume                     236.993
_cell_formula_units_Z            4
_database_code_amcsd             0003244
_diffrn_ambient_pressure         9.6e+05
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    1.999
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003155
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: r53253, T = 500 C, P = 12.3 kbar, cell volume = 234.84 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003156
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r53253, T = 500 C, P = 12.3 kbar, cell volume = 234.84 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.1696
_cell_length_b                   6.1696
_cell_length_c                   6.1696
_cell_volume                     234.839
_cell_formula_units_Z            4
_database_code_amcsd             0003245
_diffrn_ambient_pressure         1.23e+06
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    2.017
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003156
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: r55377, T = 500 C, P = 15.0 kbar, cell volume = 230.58 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003157
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r55377, T = 500 C, P = 15.0 kbar, cell volume = 230.58 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.1321
_cell_length_b                   6.1321
_cell_length_c                   6.1321
_cell_volume                     230.583
_cell_formula_units_Z            4
_database_code_amcsd             0003246
_diffrn_ambient_pressure         1.5e+06
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    2.055
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003157
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: r53197, T = 500 C, P = 18.0 kbar, cell volume = 229.09 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003158
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r53197, T = 500 C, P = 18.0 kbar, cell volume = 229.09 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.1188
_cell_length_b                   6.1188
_cell_length_c                   6.1188
_cell_volume                     229.086
_cell_formula_units_Z            4
_database_code_amcsd             0003247
_diffrn_ambient_pressure         1.8e+06
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    2.068
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003158
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: als6k80, T = 550 C, P = 0.0 kbar, cell volume = 253.30 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003159
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als6k80, T = 550 C, P = 0.0 kbar, cell volume = 253.30 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.3272
_cell_length_b                   6.3272
_cell_length_c                   6.3272
_cell_volume                     253.300
_cell_formula_units_Z            4
_database_code_amcsd             0003248
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      823.15
_exptl_crystal_density_diffrn    1.870
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003159
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: r55589, T = 550 C, P = 10.1 kbar, cell volume = 238.32 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003160
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r55589, T = 550 C, P = 10.1 kbar, cell volume = 238.32 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.1999
_cell_length_b                   6.1999
_cell_length_c                   6.1999
_cell_volume                     238.316
_cell_formula_units_Z            4
_database_code_amcsd             0003249
_diffrn_ambient_pressure         1.01e+06
_diffrn_ambient_temperature      823.15
_exptl_crystal_density_diffrn    1.988
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003160
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: r53249, T = 550 C, P = 13.3 kbar, cell volume = 234.99 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003161
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r53249, T = 550 C, P = 13.3 kbar, cell volume = 234.99 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.1709
_cell_length_b                   6.1709
_cell_length_c                   6.1709
_cell_volume                     234.988
_cell_formula_units_Z            4
_database_code_amcsd             0003250
_diffrn_ambient_pressure         1.33e+06
_diffrn_ambient_temperature      823.15
_exptl_crystal_density_diffrn    2.016
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003161
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: r55373, T = 550 C, P = 16.0 kbar, cell volume = 230.89 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003162
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r55373, T = 550 C, P = 16.0 kbar, cell volume = 230.89 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.1348
_cell_length_b                   6.1348
_cell_length_c                   6.1348
_cell_volume                     230.888
_cell_formula_units_Z            4
_database_code_amcsd             0003251
_diffrn_ambient_pressure         1.6e+06
_diffrn_ambient_temperature      823.15
_exptl_crystal_density_diffrn    2.052
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003162
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: r53201, T = 550 C, P = 18.1 kbar, cell volume = 229.49 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003163
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r53201, T = 550 C, P = 18.1 kbar, cell volume = 229.49 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.1224
_cell_length_b                   6.1224
_cell_length_c                   6.1224
_cell_volume                     229.491
_cell_formula_units_Z            4
_database_code_amcsd             0003252
_diffrn_ambient_pressure         1.81e+06
_diffrn_ambient_temperature      823.15
_exptl_crystal_density_diffrn    2.064
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003163
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: als5k80, T = 600 C, P = 0.0 kbar, cell volume = 255.85 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003164
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als5k80, T = 600 C, P = 0.0 kbar, cell volume = 255.85 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.3484
_cell_length_b                   6.3484
_cell_length_c                   6.3484
_cell_volume                     255.854
_cell_formula_units_Z            4
_database_code_amcsd             0003253
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    1.852
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003164
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: r55593, T = 600 C, P = 7.5 kbar, cell volume = 238.89 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003165
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r55593, T = 600 C, P = 7.5 kbar, cell volume = 238.89 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.2049
_cell_length_b                   6.2049
_cell_length_c                   6.2049
_cell_volume                     238.894
_cell_formula_units_Z            4
_database_code_amcsd             0003254
_diffrn_ambient_pressure         7.5e+05
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    1.983
_cod_original_cell_volume        238.893
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003165
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: r55613, T = 600 C, P = 7.5 kbar, cell volume = 241.43 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003166
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r55613, T = 600 C, P = 7.5 kbar, cell volume = 241.43 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.2268
_cell_length_b                   6.2268
_cell_length_c                   6.2268
_cell_volume                     241.432
_cell_formula_units_Z            4
_database_code_amcsd             0003255
_diffrn_ambient_pressure         7.5e+05
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    1.962
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003166
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: r53237, T = 600 C, P = 14.0 kbar, cell volume = 235.53 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003167
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r53237, T = 600 C, P = 14.0 kbar, cell volume = 235.53 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.1756
_cell_length_b                   6.1756
_cell_length_c                   6.1756
_cell_volume                     235.525
_cell_formula_units_Z            4
_database_code_amcsd             0003256
_diffrn_ambient_pressure         1.4e+06
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    2.012
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003167
_amcsd_formula_title             (K.8Na.2)Cl